WEB Quantifying Morphology of Mesoporous Materials by Electron Tomography
In previous work, we have quantitatively analyzed the morphology and the diffusion properties of a disordered mesoporous carbon material based on electron tomography. The fidelity of the segmented 3D object obtained from the Simultaneous Iterative Reconstruction Technique (SIRT) followed by image processing and with the Discrete Algebraic Reconstruction Technique (DART) is investigated using both experimental data and realistic phantoms for the material1. The CLD and skeleton analysis in Table 1 indicated that the overall morphology of these two reconstructions is similar and independent of the reconstruction methods. However, the total pore volume of the DART reconstruction differs noticeably from the segmented SIRT reconstruction, which leads to a huge difference of the simulated diffusion coefficients, as shown in figure 1c. Moreover, a phantom study based on the reconstructed mesoporous carbon indicated that the missing wedge artifacts result in a noticeable anisotropy of the diffusion coefficients in the SIRT reconstruction, while which is strongly reduced in the DART reconstruction (Figure 2), but still noticeable. This indicates that a reasonable quantitative analysis of the pore structure of a mesoporous materials using DART based electron tomography reconstructions is possible. However, despite the good performance demonstrated above, applying DART in practice is still a challenging and time consuming process, especially for the manually estimation of discrete gray values that correspond to each composition. Figure 3 showed the effect of threshold chose on the reconstructed pore volume within phantom-based SIRT and DART reconstruction. The pore volume determined from both techniques are sensitive to the threshold setting, which means trial-and-error is involved in order to achieve reasonable results. Therefore, an automatic estimation of the gray values and a better start-reconstruction with less noise and more sparse intensity for the DART reconstruction, already providing a good approximation of the morphology, is required not only for saving time but for more reliable quantification results. Currently, we are developing other reconstruction approaches as starting point for DART algorithm and extend it to other mesoporous materials for a quantitative analysis. Moreover, a deeper understanding of structure and properties for mesoporous materials is expected by combining electron tomography with bulk characterization techniques.
|Category||Short file description||File description||File Size|
|Extended Abstract||Figure 1||Figure 1. (a) Overall 3D morphology of the mesoporous carbon particle, (b) cubic substructure used for the diffusion simulations and (c) calculated effective diffusion coefficients normalized by the bulk diffusivity depending on the cube edge length for the segmented-SIRT and the DART reconstruction.||624 KB||Download|
|Extended Abstract||Figure 2||Figure 2. Effective diffusion coefficients normalized by the bulk diffusivity as a function of the simulation box size. (a) 3D, (b) x-component, (c) y-component and (d)z-component.||341 KB||Download|
|Extended Abstract||Figure3||Figure 3. Intensity histogram of a 3D reconstruction showing two main peaks corresponding to pore (void) and carbon (solid); (b) effect of threshold on the reconstructed pore volume within Phantom.segmented-SIRT and the Phantom.DART reconstructions (the dashed line indicates the pore volume of the reference phantom).||341 KB||Download|
|Extended Abstract||Table 1||Table 1. Morphological descriptors for the pore structure of the segmented-SIRT and DART reconstructions.||66 KB||Download|